# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_la2a
_database_code_depnum_ccdc_archive 'CCDC 2096805'
loop_
_audit_author_name
_audit_author_address
'Milosz Siczek'
;University of Wroclaw
Poland
;
_audit_update_record             
;
2021-07-16 deposited with the CCDC.	2022-06-05 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/1
_shelx_SHELXL_version_number     2018/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'La1.80 Mo Nd0.20 O9 W'
_chemical_formula_sum            'La1.80 Mo Nd0.20 O9 W'
_chemical_formula_weight         702.66

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      cubic
_space_group_IT_number           198
_space_group_name_H-M_alt        'P 21 3'
_space_group_name_Hall           'P 2ac 2ab 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'

_cell_length_a                   7.134(7)
_cell_length_b                   7.134(7)
_cell_length_c                   7.134(7)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     363.1(11)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    147
_cell_measurement_theta_min      4.92
_cell_measurement_theta_max      21.04

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    6.427
_exptl_crystal_F_000             605
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_exptl_absorpt_coefficient_mu    29.279
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_T_min  0.542
_exptl_absorpt_correction_T_max  0.741
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.41.80a (Rigaku Oxford Diffraction, 2020)
Numerical absorption correction based on gaussian integration over
a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Rotating-anode X-ray tube'
_diffrn_source_type              'Rigaku (Mo) X-ray Source'
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  
'XtaLAB Synergy R, DW system with HyPix-Arc 150 detector'
_diffrn_measurement_method       /w
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_type            'HyPix-Arc 150'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_reflns_number            1273
_diffrn_reflns_av_unetI/netI     0.0815
_diffrn_reflns_av_R_equivalents  0.0889
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         4.040
_diffrn_reflns_theta_max         29.876
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             348
_reflns_number_gt                242
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.626
_reflns_Friedel_fraction_max     0.957
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'CrysAlisPro 1.171.41.80a (Rigaku OD, 2020)'
_computing_cell_refinement       'CrysAlisPro 1.171.41.80a (Rigaku OD, 2020)'
_computing_data_reduction        'CrysAlisPro 1.171.41.80a (Rigaku OD, 2020)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_computing_molecular_graphics    Diamond
_computing_publication_material  'SHELXL-2018/1 (Sheldrick, 2018)'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0118P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Flack x determined using 68 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.09(11)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         348
_refine_ls_number_parameters     33
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0928
_refine_ls_R_factor_gt           0.0544
_refine_ls_wR_factor_ref         0.0700
_refine_ls_wR_factor_gt          0.0637
_refine_ls_goodness_of_fit_ref   1.056
_refine_ls_restrained_S_all      1.056
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo Mo -0.426(2) 0.074(2) -0.574(2) 0.0278(13) Uani 0.5 3 d S T P . .
La La -0.8927(4) -0.1073(4) -0.6073(4) 0.0389(8) Uani 0.9 3 d S T P . .
W W -0.3768(11) 0.081(2) -0.5630(14) 0.0278(13) Uani 0.1667 1 d . . P . .
Nd Nd -0.946(6) -0.096(11) -0.637(8) 0.0389(8) Uani 0.0333 1 d . . P . .
O1 O -0.237(3) -0.089(4) -0.567(5) 0.087(10) Uani 0.75 1 d . . P . 1
O2 O -0.210(9) 0.088(12) -0.673(10) 0.069(18) Uiso 0.25 1 d . . P . 2
O3 O -0.565(3) -0.065(3) -0.435(3) 0.093(10) Uani 1 3 d S T P . .
O4 O -0.15(2) 0.202(16) -0.59(2) 0.10(4) Uiso 0.1667 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo W 0.361(17) 11_444 ?
Mo W 0.361(17) 8_454 ?
Mo O2 1.70(7) . ?
Mo O2 1.70(7) 8_454 ?
Mo O2 1.70(7) 11_444 ?
Mo O3 1.72(5) . ?
Mo O1 1.78(2) 11_444 ?
Mo O1 1.78(2) 8_454 ?
Mo O1 1.78(2) . ?
Mo O4 2.19(16) . ?
Mo O4 2.19(16) 8_454 ?
Mo O4 2.19(16) 11_444 ?
La Nd 0.44(5) 7_344 ?
La Nd 0.44(5) 10_453 ?
La O1 2.476(19) 10_454 ?
La O1 2.476(19) 7_354 ?
La O1 2.476(19) 1_455 ?
La O4 2.56(14) 3_443 ?
La O4 2.56(14) 12_444 ?
La O4 2.56(14) 5_554 ?
La O3 2.659(11) . ?
La O3 2.659(11) 4_444 ?
La O3 2.659(11) 2_354 ?
La O2 2.70(6) 7_354 ?
W W 0.539(16) 8_454 ?
W W 0.539(16) 11_444 ?
W O2 1.43(7) . ?
W O2 1.54(7) 8_454 ?
W O1 1.57(3) . ?
W O1 1.74(3) 8_454 ?
W O2 1.77(6) 11_444 ?
W O4 1.87(16) . ?
W O3 1.93(4) . ?
W O1 2.08(2) 11_444 ?
W O4 2.15(16) 11_444 ?
W O4 2.19(16) 8_454 ?
Nd Nd 0.72(8) 10_453 ?
Nd Nd 0.72(8) 7_344 ?
Nd O1 2.13(5) 1_455 ?
Nd O2 2.31(8) 1_455 ?
Nd O1 2.40(8) 7_354 ?
Nd O3 2.42(6) 2_354 ?
Nd O1 2.45(7) 6_444 ?
Nd O4 2.51(15) 3_443 ?
Nd O4 2.58(14) 1_455 ?
Nd O3 2.61(7) 4_444 ?
Nd O1 2.69(6) 10_454 ?
Nd O4 2.72(15) 10_454 ?
O1 O4 1.54(16) 10_554 ?
O2 O4 1.10(13) . ?
O2 O4 1.43(16) 11_444 ?
O2 O2 1.77(10) 11_444 ?
O2 O2 1.77(10) 8_454 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
W Mo W 97(8) 11_444 8_454 ?
W Mo O2 59(6) 11_444 . ?
W Mo O2 95(7) 8_454 . ?
W Mo O2 95(7) 11_444 8_454 ?
W Mo O2 38(5) 8_454 8_454 ?
O2 Mo O2 63(4) . 8_454 ?
W Mo O2 38(5) 11_444 11_444 ?
W Mo O2 59(6) 8_454 11_444 ?
O2 Mo O2 63(4) . 11_444 ?
O2 Mo O2 63(4) 8_454 11_444 ?
W Mo O3 120(6) 11_444 . ?
W Mo O3 120(6) 8_454 . ?
O2 Mo O3 143(3) . . ?
O2 Mo O3 143(3) 8_454 . ?
O2 Mo O3 143(3) 11_444 . ?
W Mo O1 50(4) 11_444 11_444 ?
W Mo O1 77(2) 8_454 11_444 ?
O3 Mo O1 92.4(12) . 11_444 ?
W Mo O1 144(6) 11_444 8_454 ?
W Mo O1 50(4) 8_454 8_454 ?
O2 Mo O1 105(3) . 8_454 ?
O2 Mo O1 51(3) 8_454 8_454 ?
O2 Mo O1 106(3) 11_444 8_454 ?
O3 Mo O1 92.4(12) . 8_454 ?
O1 Mo O1 119.83(17) 11_444 8_454 ?
W Mo O1 77(2) 11_444 . ?
W Mo O1 144(6) 8_454 . ?
O3 Mo O1 92.4(12) . . ?
O1 Mo O1 119.83(17) 11_444 . ?
O1 Mo O1 119.83(17) 8_454 . ?
W Mo O4 85(7) 11_444 . ?
W Mo O4 78(6) 8_454 . ?
O2 Mo O4 29(4) . . ?
O2 Mo O4 41(3) 8_454 . ?
O2 Mo O4 74(3) 11_444 . ?
O3 Mo O4 143(3) . . ?
O1 Mo O4 124(4) 11_444 . ?
O1 Mo O4 75(4) 8_454 . ?
O1 Mo O4 66(3) . . ?
W Mo O4 78(6) 11_444 8_454 ?
W Mo O4 23(7) 8_454 8_454 ?
O2 Mo O4 74(3) . 8_454 ?
O2 Mo O4 29(4) 8_454 8_454 ?
O2 Mo O4 41(3) 11_444 8_454 ?
O3 Mo O4 143(3) . 8_454 ?
O1 Mo O4 75(4) 11_444 8_454 ?
O1 Mo O4 66(3) 8_454 8_454 ?
O1 Mo O4 124(4) . 8_454 ?
O4 Mo O4 63(6) . 8_454 ?
W Mo O4 23(7) 11_444 11_444 ?
W Mo O4 85(7) 8_454 11_444 ?
O2 Mo O4 41(3) . 11_444 ?
O2 Mo O4 74(3) 8_454 11_444 ?
O2 Mo O4 29(4) 11_444 11_444 ?
O3 Mo O4 143(3) . 11_444 ?
O1 Mo O4 66(3) 11_444 11_444 ?
O1 Mo O4 124(4) 8_454 11_444 ?
O1 Mo O4 75(4) . 11_444 ?
O4 Mo O4 63(6) . 11_444 ?
O4 Mo O4 63(6) 8_454 11_444 ?
Nd La Nd 110(9) 7_344 10_453 ?
Nd La O1 75(10) 7_344 10_454 ?
Nd La O1 36(7) 10_453 10_454 ?
Nd La O1 36(7) 7_344 7_354 ?
Nd La O1 114(8) 10_453 7_354 ?
O1 La O1 80.2(11) 10_454 7_354 ?
Nd La O1 114(8) 7_344 1_455 ?
Nd La O1 75(10) 10_453 1_455 ?
O1 La O1 80.2(11) 10_454 1_455 ?
O1 La O1 80.2(11) 7_354 1_455 ?
Nd La O4 124(10) 7_344 3_443 ?
Nd La O4 120(8) 10_453 3_443 ?
O1 La O4 154(3) 10_454 3_443 ?
O1 La O4 126(3) 7_354 3_443 ?
O1 La O4 103(3) 1_455 3_443 ?
Nd La O4 120(8) 7_344 12_444 ?
Nd La O4 78(10) 10_453 12_444 ?
O1 La O4 103(3) 10_454 12_444 ?
O1 La O4 154(3) 7_354 12_444 ?
O1 La O4 126(3) 1_455 12_444 ?
O4 La O4 53(6) 3_443 12_444 ?
Nd La O4 78(10) 7_344 5_554 ?
Nd La O4 124(10) 10_453 5_554 ?
O1 La O4 126(3) 10_454 5_554 ?
O1 La O4 103(3) 7_354 5_554 ?
O1 La O4 154(3) 1_455 5_554 ?
O4 La O4 53(6) 3_443 5_554 ?
O4 La O4 53(6) 12_444 5_554 ?
Nd La O3 53(7) 7_344 . ?
Nd La O3 79(9) 10_453 . ?
O1 La O3 64.8(8) 10_454 . ?
O1 La O3 88.0(9) 7_354 . ?
O1 La O3 144.4(10) 1_455 . ?
O4 La O3 111(3) 3_443 . ?
O4 La O3 71(3) 12_444 . ?
O4 La O3 61(3) 5_554 . ?
Nd La O3 163(10) 7_344 4_444 ?
Nd La O3 53(7) 10_453 4_444 ?
O1 La O3 88.0(9) 10_454 4_444 ?
O1 La O3 144.4(10) 7_354 4_444 ?
O1 La O3 64.8(8) 1_455 4_444 ?
O4 La O3 71(3) 3_443 4_444 ?
O4 La O3 61(3) 12_444 4_444 ?
O4 La O3 111(3) 5_554 4_444 ?
O3 La O3 116.99(14) . 4_444 ?
Nd La O3 79(9) 7_344 2_354 ?
Nd La O3 163(10) 10_453 2_354 ?
O1 La O3 144.4(10) 10_454 2_354 ?
O1 La O3 64.8(8) 7_354 2_354 ?
O1 La O3 88.0(9) 1_455 2_354 ?
O4 La O3 61(3) 3_443 2_354 ?
O4 La O3 111(3) 12_444 2_354 ?
O4 La O3 71(3) 5_554 2_354 ?
O3 La O3 116.99(13) . 2_354 ?
O3 La O3 116.99(14) 4_444 2_354 ?
Nd La O2 26(10) 7_344 7_354 ?
Nd La O2 89(7) 10_453 7_354 ?
O1 La O2 53.1(19) 10_454 7_354 ?
O1 La O2 33.1(18) 7_354 7_354 ?
O1 La O2 94.0(17) 1_455 7_354 ?
O4 La O2 149(3) 3_443 7_354 ?
O4 La O2 132(3) 12_444 7_354 ?
O4 La O2 103(3) 5_554 7_354 ?
O3 La O2 60.8(16) . 7_354 ?
O3 La O2 139.3(18) 4_444 7_354 ?
O3 La O2 95.0(19) 2_354 7_354 ?
W W W 59.999(4) 8_454 11_444 ?
W W O2 121(3) 8_454 . ?
W W O2 92(3) 11_444 . ?
W W O2 68(3) 8_454 8_454 ?
W W O2 105(4) 11_444 8_454 ?
O2 W O2 73(6) . 8_454 ?
W W O1 158(3) 8_454 . ?
W W O1 99(3) 11_444 . ?
W W O1 63(3) 8_454 8_454 ?
W W O1 123(3) 11_444 8_454 ?
O2 W O1 121(4) . 8_454 ?
O2 W O1 54(3) 8_454 8_454 ?
O1 W O1 137.2(7) . 8_454 ?
W W O2 57(3) 8_454 11_444 ?
W W O2 44(3) 11_444 11_444 ?
O2 W O2 66(4) . 11_444 ?
O2 W O2 64(4) 8_454 11_444 ?
O1 W O2 111(3) . 11_444 ?
O1 W O2 105(3) 8_454 11_444 ?
W W O4 115(4) 8_454 . ?
W W O4 121(5) 11_444 . ?
O2 W O4 36(5) . . ?
O2 W O4 49(4) 8_454 . ?
O1 W O4 78(4) . . ?
O1 W O4 86(5) 8_454 . ?
O2 W O4 82(4) 11_444 . ?
W W O3 82.0(3) 8_454 . ?
W W O3 82.0(3) 11_444 . ?
O2 W O3 149(4) . . ?
O2 W O3 138(3) 8_454 . ?
O1 W O3 91.9(13) . . ?
O1 W O3 87.0(10) 8_454 . ?
O2 W O3 123(3) 11_444 . ?
O4 W O3 156(4) . . ?
W W O1 44(2) 8_454 11_444 ?
W W O1 16(2) 11_444 11_444 ?
O1 W O1 114.3(7) . 11_444 ?
O1 W O1 107.2(6) 8_454 11_444 ?
O4 W O1 126(5) . 11_444 ?
O3 W O1 78.0(8) . 11_444 ?
W W O4 88(4) 8_454 11_444 ?
W W O4 52(3) 11_444 11_444 ?
O2 W O4 41(3) . 11_444 ?
O2 W O4 78(4) 8_454 11_444 ?
O1 W O4 81(5) . 11_444 ?
O1 W O4 130(5) 8_454 11_444 ?
O2 W O4 31(4) 11_444 11_444 ?
O4 W O4 70(6) . 11_444 ?
O3 W O4 131(3) . 11_444 ?
O1 W O4 62(3) 11_444 11_444 ?
W W O4 47(4) 8_454 8_454 ?
W W O4 78(4) 11_444 8_454 ?
O2 W O4 79(3) . 8_454 ?
O2 W O4 28(5) 8_454 8_454 ?
O1 W O4 138(4) . 8_454 ?
O1 W O4 66(3) 8_454 8_454 ?
O2 W O4 41(4) 11_444 8_454 ?
O4 W O4 69(6) . 8_454 ?
O3 W O4 128(4) . 8_454 ?
O1 W O4 70(4) 11_444 8_454 ?
O4 W O4 64(5) 11_444 8_454 ?
Nd Nd Nd 60.00(2) 10_453 7_344 ?
Nd Nd O1 103(7) 10_453 1_455 ?
Nd Nd O1 133.8(19) 7_344 1_455 ?
Nd Nd O2 131(3) 10_453 1_455 ?
Nd Nd O2 118(7) 7_344 1_455 ?
O1 Nd O2 39(2) 1_455 1_455 ?
Nd Nd O1 105(6) 10_453 7_354 ?
Nd Nd O1 60(6) 7_344 7_354 ?
O1 Nd O1 89(3) 1_455 7_354 ?
O2 Nd O1 59(3) 1_455 7_354 ?
Nd Nd O3 153(8) 10_453 2_354 ?
Nd Nd O3 97(9) 7_344 2_354 ?
O1 Nd O3 103(2) 1_455 2_354 ?
O1 Nd O3 70(2) 7_354 2_354 ?
Nd Nd O1 127(8) 10_453 6_444 ?
Nd Nd O1 144(4) 7_344 6_444 ?
O1 Nd O1 81(2) 1_455 6_444 ?
O2 Nd O1 84(2) 1_455 6_444 ?
O1 Nd O1 127(2) 7_354 6_444 ?
O3 Nd O1 62.6(17) 2_354 6_444 ?
Nd Nd O4 107(5) 10_453 3_443 ?
Nd Nd O4 110(4) 7_344 3_443 ?
O1 Nd O4 117(4) 1_455 3_443 ?
O2 Nd O4 117(4) 1_455 3_443 ?
O1 Nd O4 132(4) 7_354 3_443 ?
O3 Nd O4 65(4) 2_354 3_443 ?
O1 Nd O4 36(4) 6_444 3_443 ?
Nd Nd O4 117(4) 10_453 1_455 ?
Nd Nd O4 93(6) 7_344 1_455 ?
O1 Nd O4 54(4) 1_455 1_455 ?
O1 Nd O4 36(4) 7_354 1_455 ?
O3 Nd O4 75(4) 2_354 1_455 ?
O1 Nd O4 108(4) 6_444 1_455 ?
O4 Nd O4 136(3) 3_443 1_455 ?
Nd Nd O3 67(9) 10_453 4_444 ?
Nd Nd O3 125(9) 7_344 4_444 ?
O1 Nd O3 70.2(18) 1_455 4_444 ?
O1 Nd O3 154(2) 7_354 4_444 ?
O3 Nd O3 128(3) 2_354 4_444 ?
O1 Nd O3 65.9(18) 6_444 4_444 ?
O4 Nd O3 73(4) 3_443 4_444 ?
O4 Nd O3 124(4) 1_455 4_444 ?
Nd Nd O1 35.0(12) 10_453 10_454 ?
Nd Nd O1 60(6) 7_344 10_454 ?
O1 Nd O1 82.0(19) 1_455 10_454 ?
O2 Nd O1 98(3) 1_455 10_454 ?
O1 Nd O1 77(2) 7_354 10_454 ?
O3 Nd O1 146(3) 2_354 10_454 ?
O1 Nd O1 150(3) 6_444 10_454 ?
O4 Nd O1 142(4) 3_443 10_454 ?
O4 Nd O1 82(4) 1_455 10_454 ?
O3 Nd O1 84.7(19) 4_444 10_454 ?
Nd Nd O4 71(6) 10_453 10_454 ?
Nd Nd O4 104(5) 7_344 10_454 ?
O1 Nd O4 35(3) 1_455 10_454 ?
O2 Nd O4 62(4) 1_455 10_454 ?
O1 Nd O4 85(4) 7_354 10_454 ?
O3 Nd O4 132(4) 2_354 10_454 ?
O1 Nd O4 111(4) 6_444 10_454 ?
O4 Nd O4 139(6) 3_443 10_454 ?
O4 Nd O4 62(6) 1_455 10_454 ?
O3 Nd O4 70(4) 4_444 10_454 ?
O1 Nd O4 48(3) 10_454 10_454 ?
O4 O1 W 95(6) 10_554 . ?
O4 O1 W 111(6) 10_554 11_444 ?
W O1 W 17.8(5) . 11_444 ?
O4 O1 Mo 99(6) 10_554 . ?
W O1 Mo 10.1(9) . . ?
W O1 Mo 11.7(6) 11_444 . ?
O4 O1 W 99(6) 10_554 8_454 ?
W O1 W 5.5(6) . 8_454 ?
W O1 W 12.5(7) 11_444 8_454 ?
Mo O1 W 5.9(11) . 8_454 ?
O4 O1 Nd 94(4) 10_554 1_655 ?
W O1 Nd 130(3) . 1_655 ?
W O1 Nd 133(3) 11_444 1_655 ?
Mo O1 Nd 138(2) . 1_655 ?
W O1 Nd 132(2) 8_454 1_655 ?
O4 O1 Nd 78(5) 10_554 10_553 ?
W O1 Nd 137.3(19) . 10_553 ?
W O1 Nd 146.6(19) 11_444 10_553 ?
Mo O1 Nd 147(2) . 10_553 ?
W O1 Nd 141.3(17) 8_454 10_553 ?
Nd O1 Nd 17(2) 1_655 10_553 ?
O4 O1 Nd 74(5) 10_554 12_445 ?
W O1 Nd 107.6(18) . 12_445 ?
W O1 Nd 102.6(18) 11_444 12_445 ?
Mo O1 Nd 100(2) . 12_445 ?
W O1 Nd 105.4(17) 8_454 12_445 ?
Nd O1 Nd 122(4) 1_655 12_445 ?
Nd O1 Nd 110.8(17) 10_553 12_445 ?
O4 O1 La 87(4) 10_554 1_655 ?
W O1 La 132.1(16) . 1_655 ?
W O1 La 138.2(16) 11_444 1_655 ?
Mo O1 La 141.2(16) . 1_655 ?
W O1 La 135.3(13) 8_454 1_655 ?
Nd O1 La 7.0(15) 1_655 1_655 ?
Nd O1 La 10.2(11) 10_553 1_655 ?
Nd O1 La 118.8(19) 12_445 1_655 ?
O4 O1 Nd 85(4) 10_554 7_444 ?
W O1 Nd 123.9(16) . 7_444 ?
W O1 Nd 131.6(17) 11_444 7_444 ?
Mo O1 Nd 133.3(17) . 7_444 ?
W O1 Nd 127.4(14) 8_454 7_444 ?
Nd O1 Nd 11.2(14) 1_655 7_444 ?
Nd O1 Nd 15.1(17) 10_553 7_444 ?
Nd O1 Nd 125.8(17) 12_445 7_444 ?
La O1 Nd 8.7(10) 1_655 7_444 ?
O4 O1 La 67(5) 10_554 4_544 ?
W O1 La 110.2(12) . 4_544 ?
W O1 La 107.2(11) 11_444 4_544 ?
Mo O1 La 103.0(12) . 4_544 ?
W O1 La 108.6(9) 8_454 4_544 ?
Nd O1 La 119(2) 1_655 4_544 ?
Nd O1 La 105.9(15) 10_553 4_544 ?
Nd O1 La 7.5(14) 12_445 4_544 ?
La O1 La 114.5(10) 1_655 4_544 ?
Nd O1 La 120.9(15) 7_444 4_544 ?
O4 O1 Nd 70(5) 10_554 8_454 ?
W O1 Nd 117.8(16) . 8_454 ?
W O1 Nd 113.8(16) 11_444 8_454 ?
Mo O1 Nd 110.3(15) . 8_454 ?
W O1 Nd 116.0(14) 8_454 8_454 ?
Nd O1 Nd 112(2) 1_655 8_454 ?
Nd O1 Nd 100(2) 10_553 8_454 ?
Nd O1 Nd 11(2) 12_445 8_454 ?
La O1 Nd 107.8(12) 1_655 8_454 ?
Nd O1 Nd 114.6(15) 7_444 8_454 ?
La O1 Nd 7.9(11) 4_544 8_454 ?
O4 O2 W 94(10) . . ?
O4 O2 O4 131(10) . 11_444 ?
W O2 O4 97(6) . 11_444 ?
O4 O2 W 111(10) . 11_444 ?
W O2 W 20.4(11) . 11_444 ?
O4 O2 W 77(6) 11_444 11_444 ?
O4 O2 Mo 101(10) . . ?
W O2 Mo 8.9(7) . . ?
O4 O2 Mo 89(6) 11_444 . ?
W O2 Mo 11.6(6) 11_444 . ?
O4 O2 W 94(10) . 8_454 ?
W O2 W 15.2(8) . 8_454 ?
O4 O2 W 86(6) 11_444 8_454 ?
W O2 W 17.1(8) 11_444 8_454 ?
Mo O2 W 11.7(9) . 8_454 ?
O4 O2 O2 110(9) . 11_444 ?
W O2 O2 66(2) . 11_444 ?
O4 O2 O2 38(6) 11_444 11_444 ?
W O2 O2 50(3) 11_444 11_444 ?
Mo O2 O2 59(2) . 11_444 ?
W O2 O2 52(2) 8_454 11_444 ?
O4 O2 O2 54(10) . 8_454 ?
W O2 O2 57(3) . 8_454 ?
O4 O2 O2 95(7) 11_444 8_454 ?
W O2 O2 64(2) 11_444 8_454 ?
Mo O2 O2 59(2) . 8_454 ?
W O2 O2 48(2) 8_454 8_454 ?
O2 O2 O2 60.000(3) 11_444 8_454 ?
O4 O2 Nd 91(8) . 1_655 ?
W O2 Nd 127(5) . 1_655 ?
O4 O2 Nd 118(8) 11_444 1_655 ?
W O2 Nd 134(5) 11_444 1_655 ?
Mo O2 Nd 131(5) . 1_655 ?
W O2 Nd 142(5) 8_454 1_655 ?
O4 O2 La 87(8) . 1_655 ?
W O2 La 126(4) . 1_655 ?
O4 O2 La 122(8) 11_444 1_655 ?
W O2 La 135(5) 11_444 1_655 ?
Mo O2 La 131(4) . 1_655 ?
W O2 La 141(4) 8_454 1_655 ?
Nd O2 La 4.8(17) 1_655 1_655 ?
O4 O2 Nd 78(8) . 7_444 ?
W O2 Nd 129(4) . 7_444 ?
O4 O2 Nd 126(8) 11_444 7_444 ?
W O2 Nd 142(5) 11_444 7_444 ?
Mo O2 Nd 136(4) . 7_444 ?
W O2 Nd 144(4) 8_454 7_444 ?
O2 O2 Nd 163(5) 11_444 7_444 ?
O2 O2 Nd 131(6) 8_454 7_444 ?
Nd O2 Nd 13.5(19) 1_655 7_444 ?
La O2 Nd 9.3(10) 1_655 7_444 ?
O4 O2 La 67(10) . 3_453 ?
W O2 La 124(4) . 3_453 ?
O4 O2 La 66(8) 11_444 3_453 ?
W O2 La 118(3) 11_444 3_453 ?
Mo O2 La 121(3) . 3_453 ?
W O2 La 110(3) 8_454 3_453 ?
Nd O2 La 107(3) 1_655 3_453 ?
La O2 La 106(2) 1_655 3_453 ?
Nd O2 La 100(3) 7_444 3_453 ?
Mo O3 W 9.3(3) . 8_454 ?
Mo O3 W 9.3(3) . 11_444 ?
W O3 W 16.1(6) 8_454 11_444 ?
Mo O3 W 9.3(3) . . ?
W O3 W 16.1(6) 8_454 . ?
W O3 W 16.1(6) 11_444 . ?
Mo O3 Nd 102.4(18) . 2_355 ?
W O3 Nd 97.4(18) 8_454 2_355 ?
W O3 Nd 111.7(19) 11_444 2_355 ?
W O3 Nd 97.9(17) . 2_355 ?
Mo O3 Nd 102.4(18) . 7_344 ?
W O3 Nd 97.9(17) 8_454 7_344 ?
W O3 Nd 97.4(18) 11_444 7_344 ?
W O3 Nd 111.7(19) . 7_344 ?
Nd O3 Nd 115.5(12) 2_355 7_344 ?
Mo O3 Nd 102.4(18) . 12_445 ?
W O3 Nd 111.7(19) 8_454 12_445 ?
W O3 Nd 97.9(17) 11_444 12_445 ?
W O3 Nd 97.4(18) . 12_445 ?
Nd O3 Nd 115.5(12) 2_355 12_445 ?
Nd O3 Nd 115.5(12) 7_344 12_445 ?
Mo O3 Nd 117.4(12) . 10_453 ?
W O3 Nd 113.5(12) 8_454 10_453 ?
W O3 Nd 111.5(13) 11_444 10_453 ?
W O3 Nd 126.6(14) . 10_453 ?
Nd O3 Nd 114.1(13) 2_355 10_453 ?
Nd O3 Nd 16(2) 7_344 10_453 ?
Nd O3 Nd 104.9(14) 12_445 10_453 ?
Mo O3 Nd 117.4(13) . 5_565 ?
W O3 Nd 111.5(13) 8_454 5_565 ?
W O3 Nd 126.6(14) 11_444 5_565 ?
W O3 Nd 113.5(12) . 5_565 ?
Nd O3 Nd 16(2) 2_355 5_565 ?
Nd O3 Nd 104.9(14) 7_344 5_565 ?
Nd O3 Nd 114.1(13) 12_445 5_565 ?
Nd O3 Nd 100.5(16) 10_453 5_565 ?
Mo O3 Nd 117.4(12) . 4_544 ?
W O3 Nd 126.6(14) 8_454 4_544 ?
W O3 Nd 113.5(12) 11_444 4_544 ?
W O3 Nd 111.5(13) . 4_544 ?
Nd O3 Nd 104.9(14) 2_355 4_544 ?
Nd O3 Nd 114.1(13) 7_344 4_544 ?
Nd O3 Nd 16(2) 12_445 4_544 ?
Nd O3 Nd 100.5(16) 10_453 4_544 ?
Nd O3 Nd 100.5(16) 5_565 4_544 ?
Mo O3 La 107.9(7) . . ?
W O3 La 104.2(8) 8_454 . ?
W O3 La 102.0(7) 11_444 . ?
W O3 La 117.1(9) . . ?
Nd O3 La 119.3(13) 2_355 . ?
Nd O3 La 8.4(10) 7_344 . ?
Nd O3 La 107.6(18) 12_445 . ?
Nd O3 La 9.6(10) 10_453 . ?
Nd O3 La 107.0(16) 5_565 . ?
Nd O3 La 105.7(15) 4_544 . ?
Mo O3 La 107.9(7) . 2_355 ?
W O3 La 102.0(7) 8_454 2_355 ?
W O3 La 117.1(9) 11_444 2_355 ?
W O3 La 104.2(8) . 2_355 ?
Nd O3 La 8.4(10) 2_355 2_355 ?
Nd O3 La 107.6(18) 7_344 2_355 ?
Nd O3 La 119.3(13) 12_445 2_355 ?
Nd O3 La 105.7(15) 10_453 2_355 ?
Nd O3 La 9.6(10) 5_565 2_355 ?
Nd O3 La 107.0(16) 4_544 2_355 ?
La O3 La 111.0(7) . 2_355 ?
O2 O4 O2 88(10) . 8_454 ?
O2 O4 O1 122(10) . 7_454 ?
O2 O4 O1 144(10) 8_454 7_454 ?
O2 O4 W 50(8) . . ?
O2 O4 W 54(6) 8_454 . ?
O1 O4 W 161(7) 7_454 . ?
O2 O4 W 55(8) . 8_454 ?
O2 O4 W 41(5) 8_454 8_454 ?
O1 O4 W 174(7) 7_454 8_454 ?
W O4 W 13.2(12) . 8_454 ?
O1 O4 W 162(8) 7_454 11_444 ?
W O4 W 12.2(12) . 11_444 ?
W O4 W 14.2(11) 8_454 11_444 ?
O2 O4 Mo 49(8) . . ?
O2 O4 Mo 51(6) 8_454 . ?
O1 O4 Mo 164(7) 7_454 . ?
W O4 Mo 4.3(11) . . ?
W O4 Mo 9.5(8) 8_454 . ?
W O4 Mo 9.4(8) 11_444 . ?
O2 O4 W 162(10) . 7_454 ?
O2 O4 W 110(8) 8_454 7_454 ?
O1 O4 W 43(4) 7_454 7_454 ?
W O4 W 140(9) . 7_454 ?
W O4 W 139(8) 8_454 7_454 ?
W O4 W 151(8) 11_444 7_454 ?
Mo O4 W 142(8) . 7_454 ?
O1 O4 Nd 70(6) 7_454 3_453 ?
W O4 Nd 125(7) . 3_453 ?
W O4 Nd 115(6) 8_454 3_453 ?
W O4 Nd 114(6) 11_444 3_453 ?
Mo O4 Nd 121(6) . 3_453 ?
W O4 Nd 86(5) 7_454 3_453 ?
O1 O4 La 79(6) 7_454 3_453 ?
W O4 La 115(6) . 3_453 ?
W O4 La 106(5) 8_454 3_453 ?
W O4 La 104(5) 11_444 3_453 ?
Mo O4 La 111(6) . 3_453 ?
W O4 La 95(5) 7_454 3_453 ?
Nd O4 La 9.9(12) 3_453 3_453 ?
O1 O4 Nd 66(5) 7_454 1_655 ?
W O4 Nd 97(5) . 1_655 ?
W O4 Nd 109(5) 8_454 1_655 ?
W O4 Nd 96(5) 11_444 1_655 ?
Mo O4 Nd 100(5) . 1_655 ?
W O4 Nd 99(5) 7_454 1_655 ?
Nd O4 Nd 103(6) 3_453 1_655 ?
La O4 Nd 106(6) 3_453 1_655 ?
O2 O4 Nd 79(8) . 7_444 ?
O2 O4 Nd 164(9) 8_454 7_444 ?
O1 O4 Nd 51(4) 7_454 7_444 ?
W O4 Nd 110(5) . 7_444 ?
W O4 Nd 123(5) 8_454 7_444 ?
W O4 Nd 111(5) 11_444 7_444 ?
Mo O4 Nd 113(5) . 7_444 ?
W O4 Nd 84(5) 7_454 7_444 ?
Nd O4 Nd 100(6) 3_453 7_444 ?
La O4 Nd 105(6) 3_453 7_444 ?
Nd O4 Nd 15.4(19) 1_655 7_444 ?

_refine_diff_density_max         0.934
_refine_diff_density_min         -0.835
_refine_diff_density_rms         0.219



